## Delft University of Technology

## Weak localization in boron nitride encapsulated bilayer MoS2

Papadopoulos, Nikos; Watanabe, Kenji; Taniguchi, Takashi; Van Der Zant, Herre S.J.; Steele, Gary A. DOI

10.1103/PhysRevB.99.115414 Publication date

2019

Document Version Final published version Published in

Physical Review B

Citation (APA)

Papadopoulos, N., Watanabe, K., Taniguchi, T., Van Der Zant, H. S. J., & Steele, G. A. (2019). Weak localization in boron nitride encapsulated bilayer MoS2. Physical Review B, 99(11), [115414].

https://doi.org/10.1103/PhysRevB.99.115414 Important note

To cite this publication, please use the final published version (if applicable). Please check the document version above.

Copyright

Other than for strictly personal use, it is not permitted to download, forward or distribute the text or part of it, without the consent of the author(s) and/or copyright holder(s), unless the work is under an open content license such as Creative Commons. Takedown policy

Please contact us and provide details if you believe this document breaches copyrights. We will remove access to the work immediately and investigate your claim.

This work is downloaded from Delft University of Technology.

**Weak localization in boron nitride encapsulated bilayer MoS**

**2**

Nikos Papadopoulos,1,*_{Kenji Watanabe,}2_{Takashi Taniguchi,}2_{Herre S. J. van der Zant,}1_{and Gary A. Steele}1,†

1* _{Kavli Institute of Nanoscience, Delft University of Technology, Lorentzweg 1, Delft 2628 CJ, The Netherlands}*
2

_{National Institute for Materials Science, 1-1 Namiki, Tsukuba 305-0044, Japan}(Received 14 December 2018; revised manuscript received 21 February 2019; published 11 March 2019) We present measurements of weak localization on hexagonal boron nitride encapsulated bilayer MoS2. From

the analysis we obtain information regarding the phase coherence and the spin diffusion of the electrons. We find that the encapsulation with boron nitride provides higher mobilities in the samples, and the phase coherence shows improvement, while the spin relaxation does not exhibit any significant enhancement compared to nonencapsulated MoS2. The spin relaxation time is in the order of a few picoseconds, indicating a fast

intravalley spin-flip rate. Lastly, the spin-flip rate is found to be independent from electron density in the current range, which can be explained through counteracting spin-flip scattering processes based on electron-electron Coulomb scattering and extrinsic Bychkov-Rashba spin-orbit coupling.

DOI:10.1103/PhysRevB.99.115414

**I. INTRODUCTION**

Molybdenum disulphide (MoS2) is a member of the family of transition metal dichalcogenides (TMDCs) with semicon-ducting properties, in which the interplay between spin and other pseudospins, such as valley and layer index, has created new prospects for spintronics and valleytronics [1,2]. Bilayer MoS2is centrosymmetric and the subbands of the two K and Kvalleys are spin degenerate under nonperturbed conditions [3]. When an out-of-plane electric field is applied, an inter-layer potential is generated and the inversion symmetry breaks leading the possibility of spin-valley locking in bilayers [4–6]. Quantum corrections to the conductivity due to interfer-ence effects of charged carriers in disordered systems can pro-vide information about fundamental properties of the carriers that reside in the system [7,8]. They can, for example, provide information about the phase coherence as well as about spin [8] and other types of scattering rates of the carriers [9]. Specifically, in MoS2 and other TMDCs, weak localization (WL) or weak antilocalization (WAL) can provide crucial information about the spin lifetime established by intravalley and intervalley scattering, as well as about the Zeeman-like splitting that is induced by the intrinsic SO coupling [10,11].

Although other studies have observed WL in disordered monolayer [11] and in few-layer MoS2 samples [12,13] the case of bilayer and boron nitride encapsulated has been un-explored. In this paper, we study weak localization in high quality bilayer MoS2 encapsulated in hexagonal boron ni-tride (h-BN). Analyzing our measurements using the Hikami-Larkin-Nagaoka (HLN) model [14], we extract the spin re-laxation lengths and spin lifetimes that indicate fast spin relaxation rates through intravalley processes. Our data fur-ther suggest that the dominant source of phase decoherence is the Altshuler-Aronov-Khmelnitsky mechanism, in which

*_{n.papadopoulos@tudelft.nl}
†_{g.a.steele@tudelft.nl}

electron-electron inelastic scattering takes place [15], similar to previous studies of quantum transport in monolayer and a few-layer MoS2[11,12].

**II. RESULTS AND DISCUSSION**

Figures 1(a) and 1(b) show optical images of a van der
Waals heterostructure (sample D2) and a final device (sample
D1), respectively. To maintain the quality of MoS2 during
fabrication and to be able to establish good electrical contacts,
we followed a different route than other studies [16–18]. Prior
to the stacking of the heterostructure via the hot pick-up
technique [19], at the top h-BN sheet we opened “windows” in
*it, via standard electron beam (e-beam) lithography followed*
by reactive ion etching. This allows the metallic contacts to
be deposited directly on the MoS2channel [20], and recently
it was shown that this can be a good alternative to graphene
contacts [21]. The ohmic behavior of the current-voltage
*characteristics at moderate back-gate voltages V*g (Fig. S1)
verifies the good quality of the contacts at low temperatures
and allows the use of lock-in measurements, without the need
of complicated stacking of graphene with local gates [22,23].
In the main text we present results from data of sample D1,
while in the Supplemental Material data from sample D2 can
be found [24].

The carrier density is obtained using Hall measurements
and is found to be in the range of 4–8× 1012 cm−2 for
gate voltages between 40 and 80 V. The conductivity versus
*back-gate voltage shows typical n-type behavior and increases*
when the temperature decreases due to the metallic character
of the channel at these gate voltages [Fig. S1(b)]. As a
result of the encapsulation, the devices reach Hall
mobili-ties of∼1000 cm2*/Vs at Vg= 80 V (n = 7.9 × 10*12 cm−2)
[Fig. 1(d)] and field-effect mobilities of ∼3000 cm2_{/Vs at}*T* *= 2 K [Fig. S1(d)]. The mean free path (Le*), the diffusion
*constant (D), and the momentum relaxation time (τp*) are in
the range of 6–30 nm, 0.4–2*.2 × 10*−3m2s−1, and 55–200 fs,
respectively, assuming an effective mass of 0*.4m0, where m*0

*NIKOS PAPADOPOULOS et al.* **PHYSICAL REVIEW B 99, 115414 (2019)**

FIG. 1. A high-mobility encapsulated MoS2bilayer Hall bar and

device characteristics. (a) Optical image of an h-BN*/2L-MoS*2*/h-BN*

stack, with prepatterned holes in the top h-BN. (b) Optical image of
a completed Hall bar device. (c) Cross-sectional schematic of the
device. (d) Electrical conductivity*σ and electron mobility μ as a*
*function of the gate voltage V*g, obtained from Hall measurements at

*T* = 2 K.

is the free electron mass. Also, the Fermi level (*F*) lies in
the range of 13–24 meV above the conduction band edge.
The electron mobility increases with the carrier density, which
points to the presence of long-range Coulomb scattering [25].
The disorder induced doping in the MoS2 channel can be

*obtained by extrapolating the carrier density to zero V*g, which
*gives n*0*= 3.7 × 10*11cm−2.

At low temperatures, the magnetoresistance in our
*de-vices shows a prominent peak around B*= 0 T [Fig. 2(a)],
a clear signature of weak localization of the electron wave
functions. Figure 2(b) shows the symmetrized
magnetocon-ductivity *σ*∗*(B) [where* *σ*∗*(B)= (σ (B) + σ (−B))/2 −*
*σ (B = 0T )] in units of e*2_{/πh, for different carrier densities}*at T* = 2 K and in Fig. 2(c) for different temperatures at
*n= 7.2 × 10*12 _{cm}−2_{. As the carrier density increases, the}
dip at zero magnetic field becomes more prominent, while
it declines with temperature. The former can be attributed
to an increase of the coherence length of the electrons with
electron density, while the latter can be explained from a
decrease in the coherence as the temperature increases.
Fur-thermore, at high carrier densities the magnetoconductivities
show oscillations that are ascribed to universal conductance
fluctuations (UCFs) (see also Fig. S8). We have also observed
weak localization characteristics in the sample D2, which has
also similar transport characteristics (Fig. S2 [24]).

*For the analysis of the low B-field magnetoconductivity we*
*have employed the revised from Iordanskii et al. theory of*
Hikami-Larkin-Nagaoka [14,26,27] that has been adopted for
the analysis of magnetotransport in MoS2in previous reports
[11–13]. This model contains spin-orbit terms, responsible
for spin relaxations. We have also performed analysis with
the recent theory for monolayer TMDCs [10]. In the main
text we focus on results based on the HLN theory. The
magnetoconductivity according to the HLN model is given by
[13,14,26,27]:
*σ (B) =* *e*2
2*π*2_{¯h}*F*
*Bφ+ B*so
*B*
+1
2*F*
*Bφ+ 2B*so
*B*
−1
2*F*
*Bφ*
*B*
*.* (1)

*Here, F (z)= ψ(1/2 + z) − ln(z) and ψ is the digamma*
function. Equation (1*) contains two variables: Bφ*, which
*corresponds to the phase-coherence field and B*so, which is

FIG. 2. Weak localization in bilayer MoS2. (a) Magnetoresistivity [*ρ = ρ(B) − ρ(B = 0T), ρ(B = 0 T) = 4.56 k at V*g= 45 V] as

*a function of the back-gate voltage (V*g*) and the magnetic field (B) at T* = 2 K. The overlaid linecut shows the magnetoresistivity at a gate

*voltage of V*g*= 45 V. (b) Symmetrized magnetoconductivity σ*∗*(B) as a function of magnetic field for different electron densities n measured*

*at T* *= 2 K. (c) Symmetrized magnetoconductivity as a function of magnetic field for different temperatures with n = 7.2 × 10*12_{cm}−2_{. The}

drawn solid black lines correspond to fits using the HLN model. Data and fitted curves have been shifted vertically by 0.1e2_{/πh for clarity.}

*FIG. 3. Phase-coherence length (a) and phase-coherence time (b) as a function of the electron density for T* = 2 K. (c) Logarithmic plot
*of the phase-coherence length as a function of temperature, for two different back-gate voltages. The power law dependence with a∼ 0.5*
suggests electron-electron scattering as the dephasing mechanism.

related to the spin-orbit mediated spin relaxation processes. The black curves in Figs.2(b)and2(c)correspond to fits with Eq. (1). We have limited the fitting to fields below 1.5–2.2 T so we avoid contributions from the classical magnetoresistance and from UCFs.

From the fits, we have deduced the phase-coherence length
of the electrons. In Fig.3(a) we show the phase-coherence
*length as a function of the electron density for T* = 2 K,
*cal-culated from the relationship L _{φ}*=

*¯h/(4eB*). The error bars have been calculated based on error propagation methods. The

_{φ}*phase-coherence length is between 35 and 80 nm for n*= 5

*.5–7.5 × 10*12

_{cm}−2

_{, showing an increase with the density.}Even though the electron density is small in comparison to other reports [11–13], the phase-coherence lengths obtained here are among the largest reported for MoS2, owing to the

*large mobilities of the samples. Furthermore, values of L*obtained from weak localization data are in good agreement with the ones obtained from the conductance fluctuations: Using the equation

_{φ}*B = (¯h/e)/(πr)*2 [28] and for

*B ≈*1

*.2–2 T (period of oscillations), we get a length scale of 50–*63 nm. Another quantity that we obtain is the phase coherence

time from the relationship:*τ _{φ}= L_{φ}*2

_{/D. Figure}_{2(b)}

_{presents}the phase coherence time as a function of electron density. A weak density dependence can be observed with an increase from

*∼0.8 to ∼2 ps. Lastly, the phase coherence length is*

*found to depend on temperature with a power law: L*

_{φ}*∝ T−a*. We find values of

*α equal to 0.56 and 0.49 for Vg*= 63 V and 73 V, respectively. Such values of

*α imply dephasing due*to electron-electron scattering processes [15], which has also been reported in graphene [29], black phosphorus [28], and monolayer MoS2[11].

The fact that we observe weak localization in our devices
indicates the absence of strong disorder that leads to
inter-valley spin-flip scattering and in turn to weak
antilocaliza-tion [10,11,30]. Thus, the spin relaxation obtained through
Eq. (1) is mainly related to intravalley spin-flip processes
[Fig. 4(a)]. The dependence of the spin relaxation length
*[L*so =

√

*¯h/(4eBso*)] on density is presented in Fig. 4(b).
*The values are between 40 and 75 nm for n= 5.5 − 7.5 ×*
1012 cm−2*, exhibiting an increase with n, presumably due to*
the increase of the diffusion constant as in the case of the
phase-coherence length. The values obtained here are larger

FIG. 4. Spin relaxation properties of electrons in bilayer MoS2. (a) Energy-dispersion schematic illustrating spin relaxation due to

*intravalley spin-flip process. Different colors represent electron populations of different spin orientations. Spin relaxation length L*so(b) and

time*τ*so*(c) as a function of electron density (T*= 2 K), obtained from fitting the magnetoconductivity data to Eq. (1). The spin relaxation

*NIKOS PAPADOPOULOS et al.* **PHYSICAL REVIEW B 99, 115414 (2019)**

than the ones found in monolayer MoS2on SiO2(20 nm) [11] but somewhat smaller than those obtained from a few-layer MoS2in weak localization (100–270 nm) [12,13] and nonlo-cal spin measurements (∼200 nm) [31]. We note that the spin relaxation and phase coherence lengths seem quite similar. Although we see no reason that these should be related, it is an interesting question if there is underlying physics behind this observation.

Unlike the spin relaxation length, the spin relaxation time is
a more universal figure of merit that can be compared among
different devices and materials as it does not depend on the
diffusion constant. The spin relaxation time is found to be
relatively fast,∼2–3 ps [Fig.3(b)]. Recent reports on
pump-probe spectroscopy on monolayer WS2 have also shown fast
intravalley spin-flip rates [32]. Furthermore, we find that
the spin relaxation time is independent from the density.
We consider two counteracting effects that can explain this
observation. Firstly, according to the theoretical work of Wang
*et al. [30*] the intravalley spin-flip processes are dominated by
electron-electron Coulomb scattering. As the electron density
increases, the flip rate should thus decrease. The
spin-relaxation rate can also be tuned due to breaking of inversion
symmetry in centrosymmetric TMDCs [33,34]. The electric
field of the back gate can polarize the two layers and therefore
break the inversion symmetry of the system. In the case of our
devices though, the inversion symmetry is already broken for
the range of the back-gate voltages applied [4,35] and should
not affect the spin relaxation rate. The second mechanism
tends to increase the spin relaxation rate through the
Bychkov-Rashba SOC [36,37]. These two mechanisms could counteract
each other resulting in a relaxation time independent on
*n. For very large electric fields, the Bychkov-Rashba SOC*
dominates and the in-plane and momentum-locked effective
*B field becomes strong enough to drive the system to WAL by*
spin-flip intervalley scattering [10,13,33,38].

In addition to the HLN model that has been typically used for the analysis experiments of WL and WAL in MoS2 [11–13], a specific model was recently developed for the anal-ysis of WL and WAL in monolayer TDMCs, which takes into

account the interplay of the SO interaction and the multiple
valleys in the band structure of TMDCs [10]. The model
*developed by H. Ochoa et al. contains four free parameters*
*(B _{φ}, Bs, Be, and Bλ*). In the parameter range applicable to
our measurements, however, we find that the parameters of
the model are too strongly cross correlated to provide a
meaningful analysis of our data (see Fig. S5). We do note,
however, that with similar parameters as found in the HLN fit,
the model of Ref. [10] does provide a theoretical prediction
of the WL that is in agreement with our observations (see
Supplemental Material for the quality of the fittings as well
as results for the other fitting parameters [24]).

**III. CONCLUSION**

In summary, we have studied weak localization effects in h-BN encapsulated bilayer MoS2 devices for different temperatures and electron densities. Based on the analysis of the HLN theory, we found large phase-coherence lengths limited by electron-electron inelastic scattering. The spin relaxation rate is found to be relatively fast and independent from electron density. This latter observation may indicate the presence of counteracting relaxation mechanisms involving electron-electron scattering and spin-orbit interaction.

All raw and processed data as well as supporting code for processing and figure generation is available in Zenodo with the identifiers [39].

**ACKNOWLEDGMENTS**

This work is part of the Organization for Scientific Re-search (NWO) and the Ministry of Education, Culture, and Science (OCW). We thank Hector Ochoa and Vladimir I. Falko for their help regarding the fitting function and the localization behavior of MoS2. Growth of hexagonal boron nitride crystals was supported by the Elemental Strategy Initiative conducted by the MEXT, Japan and the CREST (JPMJCR15F3), JST.

[1] X. Xu, W. Yao, D. Xiao, and T. F. Heinz,**Nat. Phys. 10**,343

(2014).

[2] J. R. Schaibley, H. Yu, G. Clark, P. Rivera, J. S. Ross,
K. L. Seyler, W. Yao, and X. Xu, **Nat. Rev. Mater. 1**, 16055

(2016).

[3] T. Cheiwchanchamnangij and W. R. L. Lambrecht,Phys. Rev.
**B 85**,205302(2012).

[4] S. Wu, J. S. Ross, G.-B. Liu, G. Aivazian, A. Jones, Z. Fei,
W. Zhu, D. Xiao, W. Yao, D. Cobden, and X. Xu,**Nat. Phys. 9**,

149(2013).

[5] J. Lee, K. F. Mak, and J. Shan,**Nat. Nanotechnol. 11**, 421

(2016).

[6] J. Klein, J. Wierzbowski, A. Steinhoff, M. Florian, M. Rösner,
F. Heimbach, K. Müller, F. Jahnke, T. O. Wehling, J. J. Finley,
and M. Kaniber,**Nano Lett. 17**,392(2017).

[7] G. Bergmann,**Phys. Rep. 107**,1(1984).
[8] S. Kawaji,**Surf. Sci. 170**,682(1986).

[9] F. V. Tikhonenko, D. W. Horsell, R. V. Gorbachev, and A. K.
Savchenko,**Phys. Rev. Lett. 100**,056802(2008).

[10] H. Ochoa, F. Finocchiaro, F. Guinea, and V. I. Fal’ko,Phys. Rev.
**B 90**,235429(2014).

[11] H. Schmidt, I. Yudhistira, L. Chu, A. H. Castro Neto,
B. Özyilmaz, S. Adam, and G. Eda, **Phys. Rev. Lett. 116**,

046803(2016).

[12] A. T. Neal, H. Liu, J. Gu, and P. D. Ye, **ACS Nano 7**,7077

(2013).

[13] Y. J. Zhang, W. Shi, J. T. Ye, R. Suzuki, and Y. Iwasa, Phys.
**Rev. B 95**,205302(2017).

[14] S. Hikami, A. I. Larkin, and Y. Nagaoka,**Prog. Theor. Phys. 63**,

707(1980).

[15] B. L. Altshuler, A. G. Aronov, and D. E. Khmelnitsky,J. Phys.
**C: Solid State Phys. 15**,7367(1982).

[16] L. Wang, I. Meric, P. Y. Huang, Q. Gao, Y. Gao, H. Tran, T. Taniguchi, K. Watanabe, L. M. Campos, D. A. Muller,

J. Guo, P. Kim, J. Hone, K. L. Shepard, and C. R. Dean,Science

**342**,614(2013).

[17] X. Cui, G.-H. Lee, Y. D. Kim, G. Arefe, P. Y. Huang, C.-H.
Lee, D. A. Chenet, X. Zhang, L. Wang, F. Ye, F. Pizzocchero,
B. S. Jessen, K. Watanabe, T. Taniguchi, D. A. Muller, T. Low,
P. Kim, and J. Hone,**Nat. Nanotechnol. 10**,534(2015).
[18] S. Xu, Z. Wu, H. Lu, Y. Han, G. Long, X. Chen, T. Han, W. Ye,

Y. Wu, J. Lin, J. Shen, Y. Cai, Y. He, F. Zhang, R. Lortz,
C. Cheng, and N. Wang,**2D Materials 3**,021007(2016).
[19] F. Pizzocchero, L. Gammelgaard, B. S. Jessen, J. M. Caridad,

L. Wang, J. Hone, P. Bøggild, and T. J. Booth,Nat. Commun.

**7**,11894(2016).

[20] J. I.-J. Wang, Y. Yang, Y.-A. Chen, K. Watanabe, T. Taniguchi,
H. O. H. Churchill, and P. Jarillo-Herrero,**Nano Lett. 15**,1898

(2015).

[21] R. Pisoni, Z. Lei, P. Back, M. Eich, H. Overweg, Y. Lee,
K. Watanabe, T. Taniguchi, T. Ihn, and K. Ensslin,Appl. Phys.
**Lett. 112**,123101(2018).

[22] R. Pisoni, Y. Lee, H. Overweg, M. Eich, P. Simonet,
K. Watanabe, T. Taniguchi, R. Gorbachev, T. Ihn, and
K. Ensslin,**Nano Lett. 17**,5008(2017).

[23] K. Wang, K. De Greve, L. A. Jauregui, A. Sushko, A. High,
Y. Zhou, G. Scuri, T. Taniguchi, K. Watanabe, M. D. Lukin,
H. Park, and P. Kim,**Nat. Nanotechnol. 13**,128(2018).
[24] See Supplemental Material athttp://link.aps.org/supplemental/

10.1103/PhysRevB.99.115414for information about transport
*characteristics of the two devices (I*d*− V*b) traces, gate traces,

and mobilities), weak localization curves from sample D2,
*analysis of the model of Ochoa et al., and photoluminescence*
spectrum from sample D1.

[25] K. Kaasbjerg, T. Low, and A.-P. Jauho,arXiv:1612.00469. [26] S. V. Iordanskii, Yu. B. Lyanda-Geller, and G. E. Pikus, JETP

**Lett. 60, 206 (1994).**

[27] W. Knap, C. Skierbiszewski, A. Zduniak, E. Litwin-Staszewska, D. Bertho, F. Kobbi, J. L. Robert, G. E. Pikus,

F. G. Pikus, S. V. Iordanskii, V. Mosser, K. Zekentes, and Yu. B.
Lyanda-Geller,**Phys. Rev. B 53**,3912(1996).

[28] Y. Du, A. T. Neal, H. Zhou, and P. D. Ye, **2D Materials 3**,

024003(2016).

[29] R. V. Gorbachev, F. V. Tikhonenko, A. S. Mayorov, D. W.
Horsell, and A. K. Savchenko, **Phys. Rev. Lett. 98**, 176805

(2007).

[30] L. Wang and M. W. Wu,**Phys. Rev. B 89**,115302(2014).
[31] S. Liang, H. Yang, P. Renucci, B. Tao, P. Laczkowski, S.

Mc-Murtry, G. Wang, X. Marie, J.-M. George, S. Petit-Watelot,
A. Djeffal, S. Mangin, H. Jaffrès, and Y. Lu,**Nat. Commun. 8**,

14947(2017).

[32] Z. Wang, A. Molina-Sánchez, P. Altmann, D. Sangalli, D. De Fazio, G. Soavi, U. Sassi, F. Bottegoni, F. Ciccacci, M. Finazzi, L. Wirtz, A. C. Ferrari, A. Marini, G. Cerullo, and S. Dal Conte,

**Nano Lett. 18**,6882(2018).

[33] H. Yuan, M. S. Bahramy, K. Morimoto, S. Wu, K. Nomura,
B.-J. Yang, H. Shimotani, R. Suzuki, M. Toh, C. Kloc, X. Xu,
R. Arita, N. Nagaosa, and Y. Iwasa,**Nat. Phys. 9**,563(2013).
[34] A. Kormányos, V. Zólyomi, V. I. Fal’ko, and G. Burkard,Phys.

**Rev. B 98**,035408(2018).

[35] J. Lin, T. Han, B. A. Piot, Z. Wu, S. Xu, G. Long, L. An, P. Cheung, P.-P. Zheng, P. Plochocka, X. Dai, D. K. Maude, F. Zhang, and N. Wang, Nano Lett. (2019), doi:

10.1021/acs.nanolett.8b04731.

[36] H. Ochoa and R. Roldán, **Phys. Rev. B 87**, 245421

(2013).

[37] A. Kormányos, V. Zólyomi, N. D. Drummond, and G. Burkard,

**Phys. Rev. X 4**,039901(2014).

[38] L. Yang, N. A. Sinitsyn, W. Chen, J. Yuan, J. Zhang, J. Lou, and
S. A. Crooker,**Nat. Phys. 11**,830(2015).

[39] N. Papadopoulos, K. Watanabe, T. Taniguchi, H. S. J. van der Zant, and G. A. Steele, Data and codes for “Weak localization in boron nitride encapsulated bilayer MoS2”,https://doi.org/10.